Elucidation of Unsymmetrical Effect on the Piezoelectric and
Semiconducting Properties of Cd doped 1D-ZnO Nanorods
Fig. S1 Schematic representation of fabrication process of P-NG devices
The wt% value of Cd is determined by the weight ratio between Cd and Zn precursors used for
synthesis of ZnO NRs i.e., Cd(CH3COO)2·2H2O]:[Zn(CH3COO)2.2H2O]. In a typical procedure, the
molar concentration of [Zn(CH3COO)2.H2O] is taken to be 0.2 M (0.878g) and the amount of
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
This journal is © The Royal Society of Chemistry 2016
cadmium acetate dihydrate is varied as Cd/Zn = 0, 0.1, 0.5, 1, 1.5 and 2 wt%. Ex: For 1 wt% Cd
doping, 0.00878 g of Cd(CH3COO)2·2H2O] is weighed i.e.,
= 1 𝑤𝑡%
Similarly, 0.00087g and 0.00439g of Cd(CH3COO)2·2H2O] is weighed for 0.1 wt% and 0.5 wt% of
Fig. S2 Experimental flow of UV-Sensor fabrication process
Fig. S3 Growth mechanism of 1D-ZnO NRs
Fig: S3 illustrates the growth mechanism of ZnO NRs formation. The precursor dissolved in aqeous
medium forms Zn(OH)2 which undergoes two types of reaction i) it reduces to a smaller extend
forming ZnO that acts as a nucleation site ii) it form an ion-complex [Zn(OH)2-] which reacts with
HMT to form ion-pair complex or polaron (NH4+-[Zn(OH)4]2- ) due to electrostatic interaction. The
presence of NH4+ leads to rod shape morphology by orienting the polaron on c-axis of ZnO crystal.
Thus HMT acts as a surfactant by regulating the growth direction of ZnO. Sodium acetate is formed
as a by-product during the reaction between Zinc acetate dihydrate and NaOH1. Sodium acetate
formed is water soluble and therefore it gets removed during the centrifugation and heat treatment
(Please refer experimental section). Thus the final end product formed (ZnO NRs) are pure with no
impurities or by-products residing in it.
Fig. S4 XRD patterns of 1.5 wt % and 2 wt % Cd doped ZnO NRs
Fig. S5 FESEM images showing the deterioration in ZnO NRs when doped with higher Cd
concentration (a) 1.5 wt % and (b) 2 wt %
Fig. S6 Top view of FESEM images of vertically grown (a) ZnO NRs and (b) 1 wt % Cd-ZnO NRs
on glass substrate
Fig: S7. Raman spectra of undoped and 1 wt% Cd-doped ZnO NRs grown vertically on glass
Fig. S8 Cross-sectional FESEM analysis of fabricated PNG device
Fig. S9 I-V measurements at various wavelengths and illumination intensities. Undoped ZnO NRs
(a) 365 nm, (b) 405 nm (c) 535 nm and 0.5 wt% Cd-doped ZnO NRs (d) 365 nm, (e) 405 nm and (f)
Table: S1 Comparison of the Proposed UV-Sensor Device Performance with Other reports
Material Va Iph b c d Rλe Ref𝜏𝑅 𝜏𝐷
(V) (A) (s) (s) (A/W)
ZnO:Mn 5 0.2 m 2.75 16.8 0.065 2
ZnO:Ti 5 102 μ - 135 0.05 3
ZnO:Fe 8 1.13 m - - 3.66 4
ZnO:Sb 3 28.3 μ 7.3 20.3 - 5
ZnO:Mg 5 44.6 μ - - 22.33m 6
ZnO:Co 5 14 μ - - 0.0033 7
ZnO:Ag 5 40 m 80m 3.27 - 8
ZnO:C 14 - 2.97n 2.97n 1.7x106 9
ZnO:GO 10 1 μ 69 56 - 10
ZnO:Cd 10 330 μ 8 10 164m This
aBias Voltage , b Photocurrent , cResponse time, d Recovery time, ePhotoresponsivity.
Fig. S10 Schematic of SPUV-S by parallel connections between P-NG and UV-S
Fig. S11 Performance of self-powered UV-photo sensor (UV-S and UV-S1) at a wavelength of
1 J. N. Hasnidawani, H. N. Azlina, H. Norita, N. N. Bonnia, S. Ratim and E. S. Ali, Procedia
Chem., 2016, 19, 211–216.
2 C. O. Chey, X. Liu, H. Alnoor, O. Nur and M. Willander, Phys. Status Solidi - Rapid Res.
Lett., 2015, 9, 87–91.
3 P. S. Shewale, N. K. Lee, S. H. Lee, K. Y. Kang and Y. S. Yu, J. Alloys Compd., 2015, 624,
4 R. Azimirad, A. Khayatian, S. Safa and M. Almasi Kashi, J. Alloys Compd., 2014, 615,
5 W. Dai, X. Pan, S. Chen, C. Chen, W. Chen, H. Zhang and Z. Ye, RSC Adv., 2015, 5, 6311–
6 P. S. Shewale and Y. S. Yu, J. Alloys Compd., 2016, 654, 79–86.
7 H. S. Al-Salman and M. J. Abdullah, J. Mater. Sci. Technol., 2013, 29, 1139–1145.
8 Y. Liu, X. Zhang, J. Su, H. Li, Q. Zhang and Y. Gao, Opt. Express, 2014, 22, 30148–55.
9 D.-Y. Guo, C.-X. Shan, S.-N. Qu and D.-Z. Shen, Sci. Rep., 2014, 4, 7469.
10 Z. Wang, X. Zhan, Y. Wang, S. Muhammad, Y. Huang and J. He, Nanoscale, 2012, 4,